Biofunctionalization of porcine-derived collagen matrices
with platelet rich fibrin: influence on angiogenesis in vitro and in vivo
Sebastian Blatt1,2 & Valentin Burkhardt1 & Peer W. Kämmerer1 & Andreas M. Pabst3 & Keyvan Sagheb1 &
Martin Heller4 & Bilal Al-Nawas1 & Eik Schiegnitz1
Received: 25 September 2019 /Accepted: 15 January 2020
# The Author(s) 2020
Objectives Porcine-derived collagen matrices (CM) can be used for oral tissue regeneration, but sufficient revascularization is
crucial. The aim of this study was to analyze the influence of platelet-rich fibrin (PRF) on angiogenesis of different CM in vitro
and in vivo.
Materials and methods Three different CM (mucoderm®, jason®, collprotect®) were combined with PRF in a plotting process.
Growth factor release (VEGF, TGF-β) was measured in vitro via ELISA quantification after 1,4 and 7 days in comparison to PRF
alone. In ovo yolk sac (YSM) and chorion allantois membrane (CAM) model, angiogenic potential were analyzed in vivo with
light- and intravital fluorescence microscopy after 24 h, then verified with immunohistochemical staining for CD105 andαSMA.
Results Highest growth factor release was seen after 24 h for all three activated membranes in comparison to the native CM
(VEGF 24 h: each p < 0.05; TGF-β: each p < 0.001) and the PRF (no significant difference). All activated membranes revealed a
significantly increased angiogenic potential in vivo after 24 h (vessels per mm2: each p < 0.05; branching points per mm2: each p <
0.01; vessel density: each p < 0.05) andwith immunohistochemical staining for CD105 (each p < 0.01) andαSMA (each p < 0.05).
Conclusions PRF improved the angiogenesis of CM in vitro and in vivo.
Clinical relevance Bio-functionalization of CM with PRF could easily implemented in the clinical pathway and may lead to
advanced soft tissue healing.
Keywords Angiogenesis . Vascularization . Collagenmatrices . Platelet-rich fibrin . Tissue engineering
Porcine-derived collagen matrices (CM) are widely used in
oral surgery, periodontology and implantology for hard and
soft tissue regeneration . Principally, there are two different
indications in the clinical routine: on the one hand, CM can be
used as soft tissue grafts as a possible alternative to autoge-
nously connective tissue . Derived from porcine pericardi-
um, peritoneum or dorsal skin, some CM can create different
compartments for defect healing. As an occlusive barrier, they
prevent the ingrowth of gingival soft tissue into a periodontal
or bone defect and therefore allow the unimpeded prolifera-
tion and differentiation of osteogenic progenitor cells that lead
to tissue regeneration . All CM are decellularized,
deproteinized and avascular, but differ in regard to their re-
sorption process . Therefore, defect healing relies heavily
on the biomechanics of the used membrane.
Furthermore, angiogenesis and the formation of newly
formed blood vessels is mandatory to provide the required
nutritions, oxygen, immunological cells, mesenchymal stem
cells, and growth factors especially in the initial healing phase
. Problematically, the CMmight primarily exclude the new
blood vessels as well as the ingrowth of osteoprogenitor cells
from the periosteum. In order to overcome this limitation,
Electronic supplementary material The online version of this article
(https://doi.org/10.1007/s00784-020-03213-8) contains supplementary
material, which is available to authorized users.
* Sebastian Blatt
1 Department of Oral- and Maxillofacial Surgery, University Medical
Center, Augustusplatz 2, 55131 Mainz, Germany
2 Platform for Biomaterial Research, Biomatics Group, University
Medical Center, Langenbeckstrasse 1, 55131 Mainz, Germany
3 Department of Oral- and Maxillofacial Surgery, Federal Armed
Forces Hospital, Rübenacher Str. 170, 56072 Koblenz, Germany
4 Department of Gynecology, University Medical Center,
Langenbeckstrasse 1, 55131 Mainz, Germany
/ Published online: 6 February 2020
Clinical Oral Investigations (2020) 24:3425–3436
biofunctionalization of the dehydrated, acellular and avascular
CMmight lead to a optimized wound healing for example via
growth factor loading .
Autologous platelet concentrates represent a possible way
to extract the patient’s growth factors of the peripheral blood
that could be used for further biofunctionalization. Developed
as an advanced version of the fibrin sealants more than
40 years ago, nowadays different concentrates were defined
that differ in cell content and matrix architecture as well as
centrifugation process, among them Platelet- Rich Fibrin .
In this context, Park et al. modified a CM inter alia by adding
PRF and found a significantly enhanced endothelial cell mi-
gration in vitro .
Since the introduction of the PRF in 2001 by Choukroun
et al., it is widely used to support oral soft tissue regeneration
. In the literature, there is evidence that PRF can be suc-
cessfully used in the therapy of gingival recession or intrabony
defects in periodontology [10, 11], in reducing pain and swell-
ing after third molar removal , implant stability  and
other aspects of regenerative medicine [14, 15]. It is chair side
produced via specific centrifugation after venous blood col-
lection and can be processed as a liquid, injectable or stable
PRF respectively. PRF can be used as a biologically active
membrane that facilitates wound healing . Vascular
Endothelial Growth Factor (VEGF) mainly triggers the prolif-
eration and differentiation of endothelial cells. However, dif-
ferent cell-cell interactions trigger a complex interplay with
other important factors such as Transforming Growth Factor-
Beta1 (TGF-β1) and Platelet-derived Growth Factor (PDGF).
Here, mainly paracrine actions lead to the development of a
vascular system . As a result, enhanced microvessel-like
structure formation was shown when endothelial cells were
cultured with PRF in comparison to negative control . In
comparison to other autologous thrombocyte concentrates
such as Platelet Rich Plasma (PRP) the growth factor release
is described gradually and mimics physiological conditions.
As a result, the angiogenesis may initiate and tissue repair can
be optimized .
The aim of the present study was to use PRF to biologically
activate different CM.
The hypothesis was that activated membranes show similar
pro-angiogenic potential in comparison to pure PRF in vitro
and in vivo. Since differentially structured CM were used it
was secondly to be analyzed which collagen composition sup-
ports bio-activation via PRF the best.
Material and methods
Three different commercially available porcine-derived colla-
gen matrices (CM) were used: mucoderm®, jason® and
collprotect®, all: 15 × 20 mm, botiss biomaterials GmbH,
Zossen, Germany). Mucoderm® is a porcine, native, dermal
three-dimensional collagenmatrix without any artificial cross-
linking that contains natural collagen type I and III. Similarly,
collprotect® matrix represents a native, dermal three-
dimensional collagen matrix on naturally collagen and elastin
. The CM of porcine pericardium (jason®) displays inter-
connected surface system of pores .
For the PRF protocol, blood was collected from three healthy
volunteers that gave informed consent to this study. After
punction of the cephalic vein or the medial median cubital
vein,10 ml venous blood was collected with the vacutainer
system and specific sterile plain vacuum tubes with additional
silicone within their coating surface (A-PRF+, Mectron,
Carasco, Italy). Next, the collected blood was directly proc-
essed with the slow centrifugation protocol (1200 rpm for
8 min, relative centrifugal force 177 g at a fixed angle rotor
with a radius of 110 mm, Duo centrifuge, Mectron, Carasco,
Italy) as previously described . After centrifugation, the
PRF was pressed with the “PRF Box” (Mectron, Carasco,
Italy) as indicated by the manufacturer. Next, PRF was cutted
in small pieces of 16–25 mm2 and replaced in the “PRF box”.
Subsequent, the respective CM was cutted in the same sizes
and placed above the PRF, then plotted together for 30 s with-
in the box manually.
Following membranes (n = 8 each) were analyzed: JB =
activated jason® membrane, JN = native jason® membrane,
MB = activated mucoderm® membrane, MN = native
mucoderm® membrane, CB = activated collprotect® mem-
brane, CN = native collprotect® membrane, PRF = Platelet
rich fibrin and YSM= native Yolk sac membrane. The acti-
vated membranes were compared with each other, their native
equivalent as well with PRF and a negative control in the
in vivo testing. For every experiment, PRF from all three
donors were obtained, used for the activation process and
ELISA assay for in vitro quantification of growth
The respective membranes (n = 9 per respective membrane, in
total: n = 63). were cut into pieces of 0,5 square cm and trans-
ferred into 6-well plates with 2 ml of an eagle medium (Lonza,
Cologne, Germany) without growth factors under sterile con-
ditions and incubated at 37 °C and 5% CO2. After 1, 4 and
7 days the medium was changed. For each time point, 1.4 ml
of the medium was collected for further analysis and stored at